LMucko/crystallography-open-database huggingface dataset:
Halite-sylvite thermoelasticity Sample: r53053, T = 700 C, P = 16.3 kbar, cell volume = 207.86 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003253
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53053, T = 700 C, P = 16.3 kbar, cell volume = 207.86 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9237
_cell_length_b                   5.9237
_cell_length_c                   5.9237
_cell_volume                     207.864
_cell_formula_units_Z            4
_database_code_amcsd             0003342
_diffrn_ambient_pressure         1.63e+06
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    2.073
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003253
Halite-sylvite thermoelasticity Sample: r53041, T = 700 C, P = 18.0 kbar, cell volume = 206.54 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003254
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53041, T = 700 C, P = 18.0 kbar, cell volume = 206.54 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9111
_cell_length_b                   5.9111
_cell_length_c                   5.9111
_cell_volume                     206.540
_cell_formula_units_Z            4
_database_code_amcsd             0003343
_diffrn_ambient_pressure         1.8e+06
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    2.087
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003254
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r57132, T = 700 C, P = 20.6 kbar, cell volume = 205.37 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003255
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r57132, T = 700 C, P = 20.6 kbar, cell volume = 205.37 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.8999
_cell_length_b                   5.8999
_cell_length_c                   5.8999
_cell_volume                     205.369
_cell_formula_units_Z            4
_database_code_amcsd             0003344
_diffrn_ambient_pressure         2.06e+06
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    2.099
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003255
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r54474, T = 700 C, P = 22.1 kbar, cell volume = 201.80 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003256
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54474, T = 700 C, P = 22.1 kbar, cell volume = 201.80 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.8655
_cell_length_b                   5.8655
_cell_length_c                   5.8655
_cell_volume                     201.797
_cell_formula_units_Z            4
_database_code_amcsd             0003345
_diffrn_ambient_pressure         2.21e+06
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    2.136
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003256
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r57240, T = 700 C, P = 26.0 kbar, cell volume = 200.88 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003257
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r57240, T = 700 C, P = 26.0 kbar, cell volume = 200.88 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.8566
_cell_length_b                   5.8566
_cell_length_c                   5.8566
_cell_volume                     200.880
_cell_formula_units_Z            4
_database_code_amcsd             0003346
_diffrn_ambient_pressure         2.6e+06
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    2.145
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003257
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r53049, T = 750 C, P = 17.2 kbar, cell volume = 207.85 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003258
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53049, T = 750 C, P = 17.2 kbar, cell volume = 207.85 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9236
_cell_length_b                   5.9236
_cell_length_c                   5.9236
_cell_volume                     207.853
_cell_formula_units_Z            4
_database_code_amcsd             0003347
_diffrn_ambient_pressure         1.72e+06
_diffrn_ambient_temperature      1023.15
_exptl_crystal_density_diffrn    2.073
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003258
Halite-sylvite thermoelasticity Sample: b&w, T = 25 C, P = 0.0 kbar, cell volume = 200.90 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003259
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: b&w, T = 25 C, P = 0.0 kbar, cell volume = 200.90 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.3Na.7)Cl
_chemical_formula_sum            'Cl K0.3 Na0.7'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.8568
_cell_length_b                   5.8568
_cell_length_c                   5.8568
_cell_volume                     200.901
_cell_formula_units_Z            4
_database_code_amcsd             0003348
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      298.15
_exptl_crystal_density_diffrn    2.092
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.3 Na.7) Cl'
_cod_database_code               9003259
_amcsd_formula_title             (K.3Na.7)Cl
Halite-sylvite thermoelasticity Sample: als6k30, T = 508 C, P = 0.0 kbar, cell volume = 215.08 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003260
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als6k30, T = 508 C, P = 0.0 kbar, cell volume = 215.08 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.3Na.7)Cl
_chemical_formula_sum            'Cl K0.3 Na0.7'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9915
_cell_length_b                   5.9915
_cell_length_c                   5.9915
_cell_volume                     215.083
_cell_formula_units_Z            4
_database_code_amcsd             0003349
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      781.15
_exptl_crystal_density_diffrn    1.954
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.3 Na.7) Cl'
_cod_database_code               9003260
_amcsd_formula_title             (K.3Na.7)Cl
Halite-sylvite thermoelasticity Sample: als5k30, T = 550 C, P = 0.0 kbar, cell volume = 217.11 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003261
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als5k30, T = 550 C, P = 0.0 kbar, cell volume = 217.11 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.3Na.7)Cl
_chemical_formula_sum            'Cl K0.3 Na0.7'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0103
_cell_length_b                   6.0103
_cell_length_c                   6.0103
_cell_volume                     217.114
_cell_formula_units_Z            4
_database_code_amcsd             0003350
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    1.936
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.3 Na.7) Cl'
_cod_database_code               9003261
_amcsd_formula_title             (K.3Na.7)Cl
Halite-sylvite thermoelasticity Sample: als4k30, T = 600 C, P = 0.0 kbar, cell volume = 219.37 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003262
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als4k30, T = 600 C, P = 0.0 kbar, cell volume = 219.37 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.3Na.7)Cl
_chemical_formula_sum            'Cl K0.3 Na0.7'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0310
_cell_length_b                   6.0310
_cell_length_c                   6.0310
_cell_volume                     219.365
_cell_formula_units_Z            4
_database_code_amcsd             0003351
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    1.916
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.3 Na.7) Cl'
_cod_database_code               9003262
_amcsd_formula_title             (K.3Na.7)Cl
Halite-sylvite thermoelasticity Sample: als3k30, T = 650 C, P = 0.0 kbar, cell volume = 221.71 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003263
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als3k30, T = 650 C, P = 0.0 kbar, cell volume = 221.71 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.3Na.7)Cl
_chemical_formula_sum            'Cl K0.3 Na0.7'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0524
_cell_length_b                   6.0524
_cell_length_c                   6.0524
_cell_volume                     221.709
_cell_formula_units_Z            4
_database_code_amcsd             0003352
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    1.896
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.3 Na.7) Cl'
_cod_database_code               9003263
_amcsd_formula_title             (K.3Na.7)Cl
Halite-sylvite thermoelasticity Sample: b&w, T = 25 C, P = 0.0 kbar, cell volume = 193.78 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003264
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: b&w, T = 25 C, P = 0.0 kbar, cell volume = 193.78 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7868
_cell_length_b                   5.7868
_cell_length_c                   5.7868
_cell_volume                     193.783
_cell_formula_units_Z            4
_database_code_amcsd             0003353
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      298.15
_exptl_crystal_density_diffrn    2.114
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003264
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r56329, T = 350 C, P = 11.8 kbar, cell volume = 191.40 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003265
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56329, T = 350 C, P = 11.8 kbar, cell volume = 191.40 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7630
_cell_length_b                   5.7630
_cell_length_c                   5.7630
_cell_volume                     191.402
_cell_formula_units_Z            4
_database_code_amcsd             0003354
_diffrn_ambient_pressure         1.18e+06
_diffrn_ambient_temperature      623.15
_exptl_crystal_density_diffrn    2.140
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003265
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r56361, T = 350 C, P = 12.4 kbar, cell volume = 191.25 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003266
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56361, T = 350 C, P = 12.4 kbar, cell volume = 191.25 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7615
_cell_length_b                   5.7615
_cell_length_c                   5.7615
_cell_volume                     191.252
_cell_formula_units_Z            4
_database_code_amcsd             0003355
_diffrn_ambient_pressure         1.24e+06
_diffrn_ambient_temperature      623.15
_exptl_crystal_density_diffrn    2.142
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003266
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r56417, T = 350 C, P = 21.0 kbar, cell volume = 184.78 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003267
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56417, T = 350 C, P = 21.0 kbar, cell volume = 184.78 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.6958
_cell_length_b                   5.6958
_cell_length_c                   5.6958
_cell_volume                     184.784
_cell_formula_units_Z            4
_database_code_amcsd             0003356
_diffrn_ambient_pressure         2.1e+06
_diffrn_ambient_temperature      623.15
_exptl_crystal_density_diffrn    2.217
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003267
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r56325, T = 400 C, P = 12.6 kbar, cell volume = 191.86 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003268
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56325, T = 400 C, P = 12.6 kbar, cell volume = 191.86 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7676
_cell_length_b                   5.7676
_cell_length_c                   5.7676
_cell_volume                     191.860
_cell_formula_units_Z            4
_database_code_amcsd             0003357
_diffrn_ambient_pressure         1.26e+06
_diffrn_ambient_temperature      673.15
_exptl_crystal_density_diffrn    2.135
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003268
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r56413, T = 400 C, P = 21.9 kbar, cell volume = 185.01 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003269
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56413, T = 400 C, P = 21.9 kbar, cell volume = 185.01 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.6981
_cell_length_b                   5.6981
_cell_length_c                   5.6981
_cell_volume                     185.008
_cell_formula_units_Z            4
_database_code_amcsd             0003358
_diffrn_ambient_pressure         2.19e+06
_diffrn_ambient_temperature      673.15
_exptl_crystal_density_diffrn    2.214
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003269
_amcsd_formula_title             (K.2Na.8)Cl